Formability in aa5083 and aa6061 alloys for light weight applications
Materials and Design 31 (2010) S66–S70 Contents lists available at ScienceDirect Materials and Design journal homepage: www.elsevier.com/locate/matdesFormability in AA5083 and AA6061 alloys for light weight applicationsJun Liu a, Ming-Jen Tan a,*, Anders-Eric-Wollmar Jarfors b, Yingyot Aue-u-lan b, Sylvie Castagne a,ba School of Mechanical and Aerospace Engineering, Nanyang Technological University, 639798 Singapore, Singaporeb Singapore Institute of Manufacturing Technology, 638075 Singapore, Singaporea r t i c l e i n f o a b s t r a c tArticle history: With recent development in the automotive and aerospace industries, the lightweight, yet inexpensiveReceived 20 July 2009 aluminum alloys are of great demand in industrial applications. In this paper, considering the limitedAccepted 26 October 2009 applications in non-superplastic materials, two typical alloys of AA5083 and AA6061 were investigatedAvailable online 28 October 2009 and compared during high temperature tensile tests to study their formability. The results of tensile tests and microstructures were shown, which indicated the deformation properties under different conditions.Keywords: Both alloys exhibited relatively weak strain hardening effects especially at relatively lower strain rates.Aluminum alloy Furthermore, the highest strain rate sensitivity index (m value) was obtained, and the peak of percentStrain rate sensitivityMicrostructure elongation-to-failure also coincided with the ranges of highest m value. The ﬂow stress coupled with the dynamic grain growth was related with the temperatures and strain rates. The grains appeared to be coarser in the deformed samples. Cavitation and recrystallization have also been found as a result of strain rate and temperature. Ó 2009 Elsevier Ltd. All rights reserved.1. Introduction In this paper, rolled AA5083 and AA6061 were utilized as two typical non-superplastic materials and were investigated during Superplastic materials are polycrystalline solids which have the high temperature tensile tests to study their formability. The re-capability to undergo large plastic strains, often in excess of 200% sults of the tensile test coupled with optical microscopy haveprior to failure . Over past several decades, aluminum alloys been investigated, which indicate the deformation properties un-with superplasticity were widely studied for light weight applica- der different conditions. The ﬂow stress as a function of temper-tions. In order to obtain great formability and mechanical proper- ature and strain rate has been shown to establish the formabilityties, the materials with superplasticity are specially prepared. A lot of these two alloys. Furthermore, the highest strain rate sensitiv-of processing approaches including rolling, forging, extrusion, ity index (m value) is obtained to verify the feasibility of theseequal channel angular pressing (ECAP), friction stir processing two alloys. Microstructures including cavitation and recrystalliza-(FSP) and various techniques have been used to produce ﬁne tion have also been found as a result of different strain rates andrecrystallized grain size and the observation of superplasticity temperatures.[2–7]. However, those thermo-mechanical processing methodslimit the wider usage of superplastic forming (SPF) to great devel-opment due to relatively more time and higher cost . Based on 2. Experimental detailsthe limitations, a more formable material with ﬁne and stablestructure but low cost is needed, and it also expands the conven- Rolled AA5083 and AA6061 sheets with thickness of 3 mm weretional materials to be used in SPF applications. used for high temperature tensile tests and microstructure obser- Generically, the aluminum alloys of heat-treatable and high vations. Tensile specimens with 20 mm gauge length and 4 mmstrength are common used materials, such as 7075, 7475, 2024, gauge width were machined from the sheets. In order to obtain5083 and 6061 . As a commercial alloy with corrosion resistance better formability during test, all the AA5083 and AA6061 speci-and moderate to high strength, the 5083 aluminum alloy is widely mens have been annealed for 2 h at 345 °C and 415 °C, respec-applied in sheet forming processes . Additionally, the 6061 alu- tively. For AA5083, an aging treatment at 150 °C for 24 h wasminum alloy has been studied extensively because of its beneﬁts proved to be helpful to successfully reveal the microstructure bysuch as moderate strength, good formability and corrosion decorating the grain boundary with precipitates . The samplesresistance. were then mechanically polished and etched with Graf Sergeant reagent (15.5 ml HNO3, 0.5 ml HF, 3 g Cr2O3 and 84 ml H2O). For * Corresponding author. AA6061, the Poulton’s reagent-solution, (1) 50 ml solution of E-mail address: email@example.com (M.-J. Tan). 15 ml HCl, 30 ml HNO3, 2.5 ml HF and 2.5 ml H2O, (2) 25 ml0261-3069/$ - see front matter Ó 2009 Elsevier Ltd. All rights reserved.doi:10.1016/j.matdes.2009.10.052
J. Liu et al. / Materials and Design 31 (2010) S66–S70 S67 Fig. 1. Micrographs of (a) AA5083 and (b) AA6061 in the annealed condition.HNO3, (3) 40 ml of solution of 3 g chromic acid per 10 ml of dis- the curves show typical sigmoidal proﬁles. The ﬂow stress in-tilled water , was used for microstructure etching. creases with increasing strain rate. Also, the two materials differ Fig. 1 shows the typical optical microstructure of AA5083 and greatly, especially during high strain rates.AA6061 in the annealed condition. The grains were fairly equiaxed. The strain rate sensitivity index (m value), calculated fromThe grain size was measured by the linear intercept method . It slopes of the log stress vs. log strain rate (m ¼ d log r=d log e) , _is about 13.6 lm and 115 lm in average size, respectively, for are plotted in Fig. 4, respectively. The main trends for data on m va-AA5083 and AA6061. lue are as follows. Uniaxial tensile tests of the specimens were performed usingInstron 8500 testing machine equipped with an electrical resis- (1) Generally, the m value peak increases as the temperaturetance furnace chamber. The specimens were tested in the temper- increases (except AA5083) as a result of weak strain harden-ature range of 300 °C, 400 °C and 500 °C at constant crosshead ing and grain growth effects during testing at 300 °C, thedisplacement velocity, with the corresponding initial strain rate alloy has high stress at higher strain rate but low stress atfrom 0.0001 sÀ1 to 0.3 sÀ1. lower strain rate. (2) For superplastic behavior, m value would be greater than or equal to 0.3 . Unlike the superplastic materials, both3. Results and discussion AA5083 and AA6061 show the maximum values at higher strain rate. A maximum m value of 0.41 is obtained for3.1. High temperature tensile tests AA5083 at 300 °C, while 0.24 for AA6061 at 500 °C. Fig. 2 shows the true stress–strain plots for a series of initial The percent elongation-to-failure is used as a measure of thestrain rates at temperature of 300 °C. It can be observed from formability of the material and is typically a function of strain rateFig. 2, for both materials, the stress appears to increase with and temperature. The tensile elongations for both alloys plotted asdecreasing strain rate. It has been reported that the enhanced a function of log initial strain rate are shown in Fig. 5. Generally,strain hardening at slower strain rates may be because of dynamic the tensile elongation increases with increasing strain rate and testgrain growth . This can be found in AA5083, since it behaved en- temperature. This trend is different from the superplastic materialshanced strain hardening at strain rate of 10À4 sÀ1 due to great grain with slower strain rate showing larger percent elongation-to-fail-growth during high temperature deformation. However, generally ures [5–7,11]. However, the elongations do not vary a great dealthe curves exhibit relatively weak strain hardening effects espe- for different strain rates during test at 300 °C or 400 °C. That iscially at strain rates lower than 0.1 sÀ1. The curves show the similar probably due to less cavitation and weaker strain hardening effectsproﬁles at different initial stain rates under higher temperature of especially at high strain rates. There are much more cavities and400 °C or 500 °C. grain growth at 500 °C. The largest percent elongation-to-failure The ﬂow stresses as a function of strain rate at different temper- is 93.25% and 69.00%, respectively, for AA5083 and AA6061 atatures are plotted in Fig. 3. For both materials, it can be found that 500 °C. Besides, the m value confers a high resistance to neck Fig. 2. True stress–true strain tensile test curves at 300 °C and various initial strain rates of (a) AA5083 and (b) AA6061.
S68 J. Liu et al. / Materials and Design 31 (2010) S66–S70 Fig. 3. Strain rate dependence of ﬂow stress at different temperatures. Fig. 4. The m values plotted as a function of log strain rate at different temperatures. Fig. 5. Tensile percent elongation-to-failure as a function of initial strain rate at different temperatures.development and results in the high tensile elongations , so that comparing the microstructure with Fig. 7. Similar to the superplas-the maximum elongation coincides with the ranges of highest m tic materials , the alloy shows much more grain growth atvalue distributions. 500 °C. The average grain size of grip region is about 22.5 lm at 300 °C in Fig. 6a, while some of the grains grow as big as 200 lm3.2. Microstructure at 500 °C in Fig. 7a. The microstructure also contains a wide range of grain sizes, which are composed of the new, smaller grains Typical micrographs of AA5083 tested at 300 °C and initial formed due to recrystallization. It is noted that the grains havestrain rate of 10À4 sÀ1 in the grip and gauge regions are shown in higher aspect ratio along the tensile direction after testing atFig. 6. As expected, the grains appear coarser in the samples de- 300 °C.formed at high temperature due to the grain growth. The increase Cavitation has been observed in a lot of alloys including thosein grain growth caused by different temperature is evident by based on aluminum, copper, iron, lead, silver, titanium and zinc.
J. Liu et al. / Materials and Design 31 (2010) S66–S70 S69 Fig. 6. Microstructures of AA5083 tested at 300 °C and initial strain rate of 10À4 sÀ1; (a) grip and (b) gauge regions. Fig. 7. Microstructures of AA5083 tested at 500 °C and initial strain rate of 10À4 sÀ1; (a) grip and (b) gauge regions.The cavity is an internal void, which is located on the grain 1. Both the alloys exhibit relatively weaker strain hardeningboundary. Failure during deformation occurs as a result of the effects especially at relatively lower strain rates. Generally,nucleation, growth and coalescent of internal cavities . Gener- the ﬂow stress increases with increasing strain rate.ally, as an important requirement, tensile stress plays a great role 2. The m value peak increases as the temperature increases,for cavitation occurrence and growth. Little cavitation was ob- except AA5083 at 300 °C. Both AA5083 and AA6061 show theserved in the grip region from Fig. 7a because of low tensile stress maximum values at high strain rates. A maximum m value ofat this area, while much more and larger cavities were produced 0.41 is obtained for AA5083 at 300 °C, while 0.24 for AA6061in the gauge region after tensile test from Fig. 7b. It has been re- at 500 °C.ported that the failure is mostly due to internal cavitation at the 3. The largest percent elongation-to-failure is 93.25% and 69.00%,lower strain rates; but it changes to external necking at higher respectively, for AA5083 and AA6061 at 500 °C. This peak ofstrain rates . As a result, there are more cavities with the de- elongation also coincides with the range of highest m value.crease in strain rate. The fracture tip has a jagged appearance 4. The grains appear to be coarser in the samples deformed dueespecially at low strain rates. This is most likely because the sam- to the grain growth at the high temperatures. For AA5083,ple fractures along the intergranular cavities as shown in Fig. 7b. the grain size is about 13.6 lm in annealed condition, whileBesides the tensile stress, there appears to be an effect of temper- it increases to 22.5 lm at 300 °C and as big as 200 lm atature on the amount of cavitation, with higher temperature 500 °C.showing more cavitation than that of lower temperature. Com- 5. Recrystallization took place during deformation. There are moreparing the microstructures at 300 and 500 °C, it is found that cavities showing growth and coalescence of the cavities overthere are much more cavities and growth at 500 °C (Figs. 6 and time at higher temperatures and lower strain rates. The sample7). fractures along the intergranular cavities. Although neither of the two non-superplastic materials has highelongation-to-failure of superplastic materials, the relative lowﬂow stress, ductility, microstructure, temperature and strain rate Referencescan be considered for their good formability. Hence, the good form-ability could be applied by using these non-superplastic materials  Pilling J, Ridley N. Superplasticity in crystalline solids. London: The Institute ofto exploit a forming technology that does not require full Metals; 1989.  Kannan K, Vetrano JS, Hamilton CH. Effects of alloy modiﬁcation andsuperplasticity. thermomechanical processing on recrystallization of Al–Mg–Mn alloys. Metall Mater Trans A 1996;27A:2947–57.  Wu Y, Castillo LD, Lavernia EJ. Superplastic behavior of spray-deposited 5083 Al. Metall Mater Trans A 1997;28A:1059–68.  Bae DH, Ghosh AK. Grain size and temperature dependence of superplastic4. Conclusions deformation in an Al–Mg alloy under isostructural condition. Acta Mater 2000;48:1207–24. AA5083 and AA6061 specimens have been annealed for testing  Cleveland RM, Ghosh AK, Bradley JR. Comparison of superplastic behavior in two 5083 aluminum alloys. Mater Sci Eng A 2003;351:228–36.the formability at high temperatures and different strain rates. The  Kim WJ, Sa YK, Kim HK, Yoon US. Plastic forming of the equal-channel angularconclusions are summarized as follows. pressing processed 6061 aluminum alloy. Mater Sci Eng A 2008;487:360–8.
S70 J. Liu et al. / Materials and Design 31 (2010) S66–S70 Park KT, Hwang DY, Chang SY, Shin DH. Low-temperature superplastic  Verma R, Friedman PA, Ghosh AK, Kim S, Kim C. Characterization of behavior of a submicrometer-grained 5083 Al alloy fabricated by severe superplastic deformation behavior of a ﬁne grain 5083 Al alloy sheet. Metall plastic deformation. Metall Mater Trans A 2002;33A:2859–67. Mater Trans A 1996;27A:1889–98. Friedman PA, Luckey SG, Copple WB, Allor R, Miller CE, Young C. Overview of  ASM handbook, vol. 9. ASM International; 2004. superplastic forming research at ford motor company. J Mater Eng Perform  Friedman PA, Copple WB. Superplastic response in Al–Mg sheet alloys. J Mater 2004;13:670–7. Eng Perform 2004;13:335–47.